[1] | V.A. Isupov, and T.V. Kruzina, “Some physical-properties of Na0.5Bi0.5TiO3 ferroelectric.” Izv. Akad. Nauk Sssr Fiz.vol. 47, pp. 616-618, 1983. |
[2] | G.O. Jones, and P.A. Thomas, “Investigation of the structure and phase transitions in the novel A-site substituted distorted perovskite compound Na0.5Bi0.5TiO3,” Acta Crystallogr. B- Struct. Sci., vol.58, pp.168-178, 2002. |
[3] | J. R. Gomah-Pettry, S. Said, P. Marchet, and J. P. Mercurio, ‘‘Sodium-Bismuth Titanate Based Lead-Free Ferroelectric Materials,’’ J. Eur. Ceram. Soc., vol. 24 [6], pp. 1165–9, 2004. |
[4] | Y. F. Qu, D. Shan, and J. J. Song, ‘‘Effect of A-Site Substitution on Crystal Component and Dielectric Properties in Bi0.5Na0.5TiO3 Ceramics,’’ Mater. Sci. Eng., B, vol. 121 [1–2], pp. 148–51, 2005. |
[5] | Y. Hiruma, H. Nagata, and T. Takenaka, “Thermal depoling process and piezoelectric properties of bismuth sodium titanate ceramics,” J. Appl. Phys., vol. 105, pp. 084112, 2009. |
[6] | V. Dorcet, G. Trolliard, and P. Boullay, ‘‘Re-investigation of Phase Transitions in Na0.5Bi0.5TiO3 by TEM. Part I: First Order Rhombohedral to Orthorhombic Phase Transition,’’ Chem. Mater., vol. 20 [15], pp.5061–73, 2008. |
[7] | G. Trolliard and V. Dorcet, ‘‘Re-investigation of Phase Transitions in Na0.5Bi0.5TiO3 by TEM. Part II: Second Order Orthorhombic to Tetragonal Phase Transition,’’ Chem. Mater., vol. 20 [15], pp. 5074–82, 2008. |
[8] | K. Sakata and Y. Masuda, ‘‘Ferroelectric and Antiferroelectric Properties of (Na1/2 Bi1/2)TiO3–SrTiO3 Solid-Solution Ceramics,’’ Ferroelectrics, vol.7 [1–4], pp. 347–9, 1974. |
[9] | H. D. Li, C. D. Feng, and W. L. Yao, ‘‘Some Effects of Different Additives on Dielectric and Piezoelectric Properties of (Bi1/2Na1/2)TiO3–BaTiO3 Morphotropic - Phase-Boundary Composition,’’ Mater. Lett., vol. 58 [7–8], pp.1194–8, 2004. |
[10] | T. Takenaka, K. Maruyama, and K. Sakata, ‘‘(Bi1/2Na1/2)TiO3–BaTiO3 System for Lead-Free Piezoelectric Ceramics,’’ Jpn. J. Appl. Phys., Part 1, vol.30 [9B], pp. 2236–9, 1991. |
[11] | T. Oh and M. H. Kim, ‘‘Phase Relation and Dielectric Properties in (Bi1/2 Na1/2)1-xBaxTiO3 Lead-Free Ceramics,’’ Mater. Sci. Eng., B, vol.132 [3], pp. 239–46, 2006. |
[12] | L. Gao, Y. Huang, Y. Hu, and H. Du, ‘‘Dielectric and Ferroelectric Properties of (1_x)BaTiO3–(x)Bi1/2Na1/ 2TiO3 Ceramics,’’ Ceram. Int., vol.33 [6], pp. 1041–6, 2007. |
[13] | M. Chen, Q. Xu, B. H. Kim, B. K. Ahn, J. H. Ko, W. J. Kang, and O. J. Nam, ‘‘Structure and Electrical Properties of Na0.5Bi0.5)1-xBaxTiO3 Piezoelectric Ceramics,’’ J. Eur. Ceram. Soc., vol.28 [4], pp. 843–9, 2008. |
[14] | Y. Q. Huang, L. F. Gao, Y. Hu, and H. Y. Du, ‘‘Compositional Effects on the Properties of (1_x) BaTiO3–xBi0.5Na0.5TiO3 Ceramics,’’ J. Mater. Sci.: Mater. Electron., vol.18 [6],pp. 605–9, 2007. |
[15] | Y. Hosono, K. Harada, and Y. Yamashita, ‘‘Crystal Growth and Electrical Properties of Lead-Free Piezoelectric Material (Na1/2Bi1/2)TiO3–BaTiO3,’’ Jpn. J. Appl. Phys., Part 1, vol.40 [9B], pp. 5722–6, 2001. |
[16] | O. Elkechai, M. Manier, and J. P. Mercurio, ‘‘Na0.5Bi0.5TiO3–K0.5Bi0.5TiO3 (NBT–KBT) System: A Structural and Electrical Study,’’ Phys. Status Solidi A, vol. 157 [2], pp. 499–506, 1996. |
[17] | Y. Yamada, T. Akutsu, H. Asada, K. Nozawa, S. Hachiga, T. Kurosaki, O. Ikagawa, H. Fujiki, K. Hozumi, T. Kawamura, T. Amakawa, K. Hirota, and T. Ikeda, ‘‘Effect of B-Ions Substitution in [(K1/2Bi1/2)–(Na1/2Bi1/2)](Ti–B)O3 System with B5Zr, Fe1/2Nb1/2, Zn1/3Nb2/3 or Mg1/3Nb2/ 3,’’ Jpn. J. Appl. Phys., Part 1, vol.34 [9B], pp.5462–6, 1995. |
[18] | A. Sasaki, T. Chiba, Y. Mamiya, and E. Otsuki, ‘‘Dielectric and Piezoelectric Properties of (Bi1/2Na1/2)TiO3 – (Bi0.5K0.5)TiO3 Systems,’’ Jpn. J. Appl. Phys., Part 1, vol.38 [9B], pp.5564–7, 1999. |
[19] | Z. Yang, B. Liu, L. Wei, and Y. Hou, ‘‘Structure and Electrical Properties of (1_x) Bi0.5Na0.5TiO3 – xBi0.5K0.5TiO3 Ceramics Near Morphotropic Phase Boundary,’’ Mater. Res. Bull., vol. 43 [1], pp.81–89, 2008. |
[20] | K. Yoshii, Y. Hiruma, H. Nagata, and T. Takenaka, ‘‘Electrical Properties and Depolarization Temperature of (Bi1/2Na1/2)TiO3–(Bi1/2K1/2)TiO3 Lead-Free Piezoelectric Ceramics,’’ Jpn. J. Appl. Phys., Part 1, 45 [5B], pp. 4493–6, 2006. |
[21] | Y. Makiuchi, R. Aoyagi, Y. Hiruma, H. Nagata, and T. Takenaka, ‘‘(Bi1/2 Na1/2)TiO3–(Bi1/2K1/2)TiO3–BaTiO3 - Based Lead-Free Piezoelectric Ceramics,’’ Jpn. J. Appl. Phys., Part 1,vol. 44 [6B], pp. 4350–3, 2005. |
[22] | X. X. Wang, H. L. W. Chan, and C. L. Choy, ‘‘(Bi1/2Na1/2)TiO3–Ba (Cu1/2W1/2)O3 Lead-Free Piezoelectric Ceramics,’’ J. Am. Ceram. Soc., vol.86 [10], pp. 1809–11, 2003. |
[23] | J. Shieh, K. C. Wu, and C. S. Chen, ‘‘Switching Characteristics of MPB Compositions of (Bi0.5Na0.5)TiO3 – BaTiO3–(Bi0.5K0.5)TiO3 Lead-Free Ferroelectric Ceramics,’’ Acta Mater., vol. 55 [9], pp. 3081–7, 2007. |
[24] | W. Chen, Y. M. Li, Q. Xu, and J. Zhou, ‘‘Electromechanical Properties and Morphotropic Phase Boundary of Na0.5Bi0.5TiO3–K0.5Bi0.5TiO3–BaTiO3 Lead-Free Piezoelectric Ceramics,’’ J. Electroceram., vol.15 [3], pp. 229–35, 2005. |
[25] | X. X. Wang, S. H. Choy, X. G. Tang, and H. L. W. Chan, ‘‘Dielectric Behavior and Microstructure of (Bi1/2Na1/2)TiO3–(Bi1/2K1/2)TiO3–BaTiO3 Lead-Free Piezoelectric Ceramics,’’ J. Appl. Phys., vol.97 [10], pp. 104101, 2005. |
[26] | S. H. Choy, X. X. Wang, C. P. Chong, H. L. W. Chan, P. C. K. Liu, and C. L. Choy, ‘‘0.90(Bi1/2Na1/2)TiO3 – 0.05(Bi1/2K1/2)TiO3–0.05BaTiO3 Transducer for Ultrasonic Wirebonding Applications,’’ Appl. Phys. A: Mater. Sci. Process., vol.84 [3], 313–6, 2006. |
[27] | Y. Hiruma, H. Nagata, and T. Takenaka, ‘‘Phase-Transition Temperatures and Piezoelectric Properties of (Bi1/2Na1/2)TiO3–(Bi1/2Li1/2)TiO3–(Bi1/2K1/2)TiO3 Lead-Free Ferroelectric Ceramics,’’ IEEE Trans. Ultrason. Ferroelectr. Freq. Control, vol.54 [12], pp. 2493–9, 2007. |
[28] | Jasneet Kaur, Vinay Gupta, R. K. Kotnala, Kuldeep Chandra Verma, Size dependent dielectric properties of Co and Fe doped SnO_{2} nanoparticles and their nanorods by Ce co-doping, Indian JHournal of Pure & Applied Physics, vol.50, pp. 57-63, 2012. |
[29] | F. Kremer, A. Schönhals, Broadband Dielectric Spectroscopy, Germany: Springer-Verlag, pp.476, 2003. |
[30] | T. Gopal Reddy, B. Rajesh Kumar, T. Subba Rao, and J. Altaf Ahmad, “Structural and dielectric properties of barium bismuth titanate (BaBi4Ti4O15) ceramics,” International Journal of Applied Engineering Research, vol. 6, no. 5, pp. 571–580, 2011. |
[31] | Pharatree Jaita, Anucha Watcharapasorn, Nitish Kumar, David P. Cann, and Sukanda Jiansirisomboon,” Large Electric Field-Induced Strain and Piezoelectric Responses of Lead-FreeBi0.5(Na0.80K0.20)0.5TiO3-Ba(Ti0.90Sn0.10)O3 Ceramics Near Morphotropic Phase Boundary,” Electron. Mater. Lett., Vol. 11(5), pp.828-835, 2015. |
[32] | D.C. Sinclair, and A.R. West, “Impedance and modulus spectroscopy of semiconducting BaTiO_{3} showing positive temperature coefficient of resistance,” Journal of Applied Physics, vol. 66, pp. 3850-3856, 1989. |
[33] | D.C. Sinclair, and A.R. West, “Effect of atmosphere on the PTCR properties of BaTiO_{3} ceramics,” Journal of Materials Science, vol.29, pp.6061-6068, 1994. |
[34] | O. A. Tsagareishvili, L. S. Chkhartishvili, D. L. Gabunia, “Apparent low-frequency charge capacitance of semiconducting boron,” Semiconductors, vol.43[1], pp.14-20, 2009. |
[35] | M. Widom, M. Mihalkovic, “Relative stability of α and β boron. Journal of Physics: Conference Series,” vol.176, 012024, pp. 1-10, 2009. |
[36] | K. Sambasiva Rao, K. Varada Rajuluua, B. Tilak, and A. Swathi, “Effect of Ba^{2+} in BNT ceramics on dielectric and conductivity properties,” Natural Science, vol. 2 (4), pp.357-367, 2010. |
[37] | M.C. Steil, F. Thevenot, and M. Kleitz, “Densification of yttria‐stabilized zirconia: impedance spectroscopy analysis,” Journal of Electrochemical Society, vol.144, pp.390-398, 1997. |
[38] | H. D. Li, C. D. Feng, and P. H. Xiang, “Electrical properties of La^{3+} doped Na_{0.5}Bi_{0.5})_{0.94}Ba_{0.06}TiO_{3} ceramics,” Jpn. J. Appl. Phys., vol.42, pp.7387–7391, 2003. |
[39] | Ruzhong Zuo, Hongqiang Wang, Bing Ma,and Longtu Li, “Effects of Nb^{5+} doping on sintering and electrical properties of lead-free (Bi0.5Na0.5)TiO3 ceramics” J. Mater Sci: Mater Electron, vol. 20, pp.1140–1143 DOI 10.1007/s 10854-008- 9840-9, 2009. |
[40] | Sambasiva Rao K, Varada Rajuluua K, Tilak B, A Swathi, “Effect of Ba2+ in BNT ceramics on dielectric and conductivity properties,” Natural Science, vol. 2 (4), pp.357, 2010. |
[41] | F. A.Kröger and H. J.Vink, “Relations between the concentrations of imperfections in crystalline solids,” Solid State Phys, vol. 3, pp. 307-435, 1956. |
[42] | M. J. Forbess, S. Seraji, Y. Wu, C. P. Nguyen, and G. Z. Cao, “Dielectric properties of layered perovskite Sr_{1−}_{x}A_{x}Bi_{2}Nb_{2}O_{9} ferroelectrics (A=La, Ca and x = 0, 0.1),” Applied Physics Letters, vol.76(20), pp.2934–2936, 2000. |
[43] | K. Funke, “Jump relaxation in solid electrolytes,” Progress in Solid State Chemistry, vol. 22(2), pp. 111–195, 1993. |
[44] | S. R. Elliot, “AC conduction in amorphous chalcogenide and pnictide semiconductors,” Advances in Physics, vol.36, pp.135–217, 1987. |
[45] | N. Ortega, A. Kumar, P. Bhattacharya, S.B. Majumdar, and R.S. Katiyar, “Impedance spectroscopy of multiferroic PbZr_{x}Ti_{1-x}O_{3}/CoFe_{2}O_{4} layered thin films,” Physical Review B, vol.77, pp.014111-014120, 2008. |
[46] | D. Emin, “Optical properties of large and small polarons and bipolarons,” Physical Review B, vol.48(18), pp.13691-13702, 1993. |